DOI: 10.17188/1697765
title: Materials Data on Li4V3P8O29 by Materials Project

description: Li4V3P8O29 crystallizes in the triclinic P1 space group. The structure is three-dimensional. there are eight inequivalent Li1+ sites. In the first Li1+ site, Li1+ is bonded to four O2- atoms to form distorted LiO4 tetrahedra that share corners with four PO4 tetrahedra and an edgeedge with one VO6 octahedra. There are a spread of Li–O bond distances ranging from 1.99–2.13 Å. In the second Li1+ site, Li1+ is bonded in a 4-coordinate geometry to four O2- atoms. There are a spread of Li–O bond distances ranging from 1.92–2.34 Å. In the third Li1+ site, Li1+ is bonded in a 5-coordinate geometry to five O2- atoms. There are a spread of Li–O bond distances ranging from 1.90–2.74 Å. In the fourth Li1+ site, Li1+ is bonded to four O2- atoms to form distorted LiO4 tetrahedra that share corners with four PO4 tetrahedra and an edgeedge with one VO6 octahedra. There are a spread of Li–O bond distances ranging from 1.96–2.11 Å. In the fifth Li1+ site, Li1+ is bonded in a 4-coordinate geometry to five O2- atoms. There are a spread of Li–O bond distances ranging from 1.91–2.75 Å. In the sixth Li1+ site, Li1+ is bonded in a 4-coordinate geometry to four O2- atoms. There are a spread of Li–O bond distances ranging from 1.92–2.36 Å. In the seventh Li1+ site, Li1+ is bonded in a 2-coordinate geometry to five O2- atoms. There are a spread of Li–O bond distances ranging from 1.95–2.58 Å. In the eighth Li1+ site, Li1+ is bonded in a 5-coordinate geometry to five O2- atoms. There are a spread of Li–O bond distances ranging from 1.97–2.55 Å. There are six inequivalent V+4.67+ sites. In the first V+4.67+ site, V+4.67+ is bonded to six O2- atoms to form VO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of V–O bond distances ranging from 1.86–1.91 Å. In the second V+4.67+ site, V+4.67+ is bonded to six O2- atoms to form VO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of V–O bond distances ranging from 1.85–1.94 Å. In the third V+4.67+ site, V+4.67+ is bonded to six O2- atoms to form VO6 octahedra that share corners with six PO4 tetrahedra and an edgeedge with one LiO4 tetrahedra. There are a spread of V–O bond distances ranging from 1.92–2.03 Å. In the fourth V+4.67+ site, V+4.67+ is bonded to six O2- atoms to form VO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of V–O bond distances ranging from 1.83–1.97 Å. In the fifth V+4.67+ site, V+4.67+ is bonded to six O2- atoms to form VO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of V–O bond distances ranging from 1.83–1.97 Å. In the sixth V+4.67+ site, V+4.67+ is bonded to six O2- atoms to form VO6 octahedra that share corners with six PO4 tetrahedra and an edgeedge with one LiO4 tetrahedra. There are a spread of V–O bond distances ranging from 1.85–2.04 Å. There are sixteen inequivalent P5+ sites. In the first P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra, a cornercorner with one LiO4 tetrahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 40–46°. There are a spread of P–O bond distances ranging from 1.50–1.63 Å. In the second P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 36–42°. There are a spread of P–O bond distances ranging from 1.47–1.62 Å. In the third P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra, a cornercorner with one LiO4 tetrahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 35–37°. There are a spread of P–O bond distances ranging from 1.48–1.61 Å. In the fourth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with three VO6 octahedra. The corner-sharing octahedra tilt angles range from 29–32°. There are a spread of P–O bond distances ranging from 1.48–1.59 Å. In the fifth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with three VO6 octahedra and a cornercorner with one LiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 34–38°. There are a spread of P–O bond distances ranging from 1.50–1.61 Å. In the sixth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra, a cornercorner with one LiO4 tetrahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 36–40°. There are a spread of P–O bond distances ranging from 1.50–1.61 Å. In the seventh P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra, a cornercorner with one LiO4 tetrahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 38–40°. There are a spread of P–O bond distances ranging from 1.50–1.60 Å. In the eighth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 39–40°. There are a spread of P–O bond distances ranging from 1.50–1.60 Å. In the ninth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra, a cornercorner with one LiO4 tetrahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 35–36°. There are a spread of P–O bond distances ranging from 1.48–1.61 Å. In the tenth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 37–38°. There are a spread of P–O bond distances ranging from 1.50–1.62 Å. In the eleventh P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 37–38°. There are a spread of P–O bond distances ranging from 1.50–1.62 Å. In the twelfth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with three VO6 octahedra. The corner-sharing octahedra tilt angles range from 29–32°. There are a spread of P–O bond distances ranging from 1.48–1.60 Å. In the thirteenth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with three VO6 octahedra and a cornercorner with one LiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 33–37°. There are a spread of P–O bond distances ranging from 1.49–1.60 Å. In the fourteenth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 39–40°. There are a spread of P–O bond distances ranging from 1.50–1.60 Å. In the fifteenth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra, a cornercorner with one LiO4 tetrahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 37–46°. There are a spread of P–O bond distances ranging from 1.50–1.64 Å. In the sixteenth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 36–42°. There are a spread of P–O bond distances ranging from 1.47–1.62 Å. There are fifty-eight inequivalent O2- sites. In the first O2- site, O2- is bonded in a 3-coordinate geometry to two Li1+ and one P5+ atom. In the second O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one V+4.67+, and one P5+ atom. In the third O2- site, O2- is bonded in a 3-coordinate geometry to two Li1+ and one P5+ atom. In the fourth O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one V+4.67+, and one P5+ atom. In the fifth O2- site, O2- is bonded in a bent 150 degrees geometry to one V+4.67+ and one P5+ atom. In the sixth O2- site, O2- is bonded in a bent 150 degrees geometry to one V+4.67+ and one P5+ atom. In the seventh O2- site, O2- is bonded in a bent 150 degrees geometry to one V+4.67+ and one P5+ atom. In the eighth O2- site, O2- is bonded in a bent 150 degrees geometry to one Li1+ and one P5+ atom. In the ninth O2- site, O2- is bonded in a bent 150 degrees geometry to one V+4.67+ and one P5+ atom. In the tenth O2- site, O2- is bonded in a bent 150 degrees geometry to one V+4.67+ and one P5+ atom. In the eleventh O2- site, O2- is bonded in a bent 150 degrees geometry to one V+4.67+ and one P5+ atom. In the twelfth O2- site, O2- is bonded in a distorted trigonal non-coplanar geometry to one Li1+, one V+4.67+, and one P5+ atom. In the thirteenth O2- site, O2- is bonded in a single-bond geometry to one P5+ atom. In the fourteenth O2- site, O2- is bonded in a distorted single-bond geometry to one Li1+ and one P5+ atom. In the fifteenth O2- site, O2- is bonded in a bent 150 degrees geometry to one V+4.67+ and one P5+ atom. In the sixteenth O2- site, O2- is bonded in a bent 150 degrees geometry to one V+4.67+ and one P5+ atom. In the seventeenth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one V+4.67+, and one P5+ atom. In the eighteenth O2- site, O2- is bonded in a bent 150 degrees geometry to one V+4.67+ and one P5+ atom. In the nineteenth O2- site, O2- is bonded in a distorted bent 150 degrees geometry to two P5+ atoms. In the twentieth O2- site, O2- is bonded in a distorted trigonal planar geometry to two Li1+ and one P5+ atom. In the twenty-first O2- site, O2- is bonded in a distorted trigonal planar geometry to two Li1+ and one P5+ atom. In the twenty-second O2- site, O2- is bonded in a bent 150 degrees geometry to one V+4.67+ and one P5+ atom. In the twenty-third O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one V+4.67+, and one P5+ atom. In the twenty-fourth O2- site, O2- is bonded in a bent 150 degrees geometry to one V+4.67+ and one P5+ atom. In the twenty-fifth O2- site, O2- is bonded in a bent 150 degrees geometry to one V+4.67+ and one P5+ atom. In the twenty-sixth O2- site, O2- is bonded in a bent 150 degrees geometry to one V+4.67+ and one P5+ atom. In the twenty-seventh O2- site, O2- is bonded in a distorted bent 150 degrees geometry to two P5+ atoms. In the twenty-eighth O2- site, O2- is bonded in a bent 150 degrees geometry to one Li1+ and one P5+ atom. In the twenty-ninth O2- site, O2- is bonded in a 3-coordinate geometry to two Li1+ and one P5+ atom. In the thirtieth O2- site, O2- is bonded in a bent 150 degrees geometry to one V+4.67+ and one P5+ atom. In the thirty-first O2- site, O2- is bonded in a bent 150 degrees geometry to one V+4.67+ and one P5+ atom. In the thirty-second O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one V+4.67+, and one P5+ atom. In the thirty-third O2- site, O2- is bonded in a bent 150 degrees geometry to one V+4.67+ and one P5+ atom. In the thirty-fourth O2- site, O2- is bonded in a bent 150 degrees geometry to one V+4.67+ and one P5+ atom. In the thirty-fifth O2- site, O2- is bonded in a distorted trigonal planar geometry to two Li1+ and one P5+ atom. In the thirty-sixth O2- site, O2- is bonded in a distorted trigonal planar geometry to two Li1+ and one P5+ atom. In the thirty-seventh O2- site, O2- is bonded in a bent 120 degrees geometry to two P5+ atoms. In the thirty-eighth O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one V+4.67+, and one P5+ atom. In the thirty-ninth O2- site, O2- is bonded in a distorted trigonal non-coplanar geometry to one